#------------------------------------------------------------------------------
#$Date: 2016-03-26 16:48:11 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180356 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/25/7202515.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7202515
loop_
_publ_author_name
'Galati, Rosa'
'Hughes, Robert W.'
'Knee, Christopher S.'
'Henry, Paul F.'
'Weller, Mark T.'
_publ_section_title
;
 The structure of superconducting RbOs2O6 between 2 K and 300 K
;
_journal_issue                   2
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              160
_journal_paper_doi               10.1039/b613083f
_journal_volume                  17
_journal_year                    2007
_chemical_formula_sum            'O6 Os2 Rb'
_chemical_formula_weight         561.86
_chemical_name_common            '300K Fd3M'
_chemical_name_systematic        ' ?'
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_audit_creation_date             2006-10-10T17:37
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2006-10-10T17:37 Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            8
_cell_length_a                   10.11393(5)
_cell_length_b                   10.11393
_cell_length_c                   10.11393
_cell_measurement_temperature    300
_cell_volume                     1034.570(5)
_computing_structure_refinement  GSAS
_pd_block_id                     2006-10-10T17:37|FULL_ANI|RW_Hughes|D2B
_pd_char_colour                  black
_pd_phase_name                   '300K Fd3M'
_pd_prep_conditions
;Heated at 100K/hour to 873.
Held for 14 hours. Furnace cooled.
;
_pd_prep_temperature             873
_refine_ls_goodness_of_fit_all   1.09
_refine_ls_matrix_type           full
_refine_ls_number_parameters     16
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.01
_refine_ls_shift/su_mean         0.00
_cod_data_source_file            b613083f.txt
_cod_data_source_block           FULL_ANI_publ
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (63
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (51 time).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        1034.569(17)
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               7202515
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 +z,+x,+y
3 +y,+z,+x
4 +x+1/4,+y+1/4,-z
5 -z,+x+1/4,+y+1/4
6 +y+1/4,-z,+x+1/4
7 -z+1/4,+x+1/2,-y+3/4
8 -y+3/4,-z+1/4,+x+1/2
9 +y+1/2,-z+1/4,-x+3/4
10 -x+3/4,+y+1/2,-z+1/4
11 -z+1/4,-x+3/4,+y+1/2
12 +x+1/2,-y+3/4,-z+1/4
13 +y,+x,+z
14 +z,+y,+x
15 +x,+z,+y
16 +y+1/4,+x+1/4,-z
17 -z,+y+1/4,+x+1/4
18 +x+1/4,-z,+y+1/4
19 -z+1/4,+y+1/2,-x+3/4
20 -x+3/4,-z+1/4,+y+1/2
21 +x+1/2,-z+1/4,-y+3/4
22 -y+3/4,+x+1/2,-z+1/4
23 -z+1/4,-y+3/4,+x+1/2
24 +y+1/2,-x+3/4,-z+1/4
-1 -x,-y,-z
-2 -z,-x,-y
-3 -y,-z,-x
-4 -x+3/4,-y+3/4,+z
-5 +z,-x+3/4,-y+3/4
-6 -y+3/4,+z,-x+3/4
-7 +z+3/4,-x+1/2,+y+1/4
-8 +y+1/4,+z+3/4,-x+1/2
-9 -y+1/2,+z+3/4,+x+1/4
-10 +x+1/4,-y+1/2,+z+3/4
-11 +z+3/4,+x+1/4,-y+1/2
-12 -x+1/2,+y+1/4,+z+3/4
-13 -y,-x,-z
-14 -z,-y,-x
-15 -x,-z,-y
-16 -y+3/4,-x+3/4,+z
-17 +z,-y+3/4,-x+3/4
-18 -x+3/4,+z,-y+3/4
-19 +z+3/4,-y+1/2,+x+1/4
-20 +x+1/4,+z+3/4,-y+1/2
-21 -x+1/2,+z+3/4,+y+1/4
-22 +y+1/4,-x+1/2,+z+3/4
-23 +z+3/4,+y+1/4,-x+1/2
-24 -y+1/2,+x+1/4,+z+3/4
101 +x,+y+1/2,+z+1/2
102 +z,+x+1/2,+y+1/2
103 +y,+z+1/2,+x+1/2
104 +x+1/4,+y+3/4,-z+1/2
105 -z,+x+3/4,+y+3/4
106 +y+1/4,-z+1/2,+x+3/4
107 -z+1/4,+x,-y+1/4
108 -y+3/4,-z+3/4,+x
109 +y+1/2,-z+3/4,-x+1/4
110 -x+3/4,+y,-z+3/4
111 -z+1/4,-x+1/4,+y
112 +x+1/2,-y+1/4,-z+3/4
113 +y,+x+1/2,+z+1/2
114 +z,+y+1/2,+x+1/2
115 +x,+z+1/2,+y+1/2
116 +y+1/4,+x+3/4,-z+1/2
117 -z,+y+3/4,+x+3/4
118 +x+1/4,-z+1/2,+y+3/4
119 -z+1/4,+y,-x+1/4
120 -x+3/4,-z+3/4,+y
121 +x+1/2,-z+3/4,-y+1/4
122 -y+3/4,+x,-z+3/4
123 -z+1/4,-y+1/4,+x
124 +y+1/2,-x+1/4,-z+3/4
-101 -x,-y+1/2,-z+1/2
-102 -z,-x+1/2,-y+1/2
-103 -y,-z+1/2,-x+1/2
-104 -x+3/4,-y+1/4,+z+1/2
-105 +z,-x+1/4,-y+1/4
-106 -y+3/4,+z+1/2,-x+1/4
-107 +z+3/4,-x,+y+3/4
-108 +y+1/4,+z+1/4,-x
-109 -y+1/2,+z+1/4,+x+3/4
-110 +x+1/4,-y,+z+1/4
-111 +z+3/4,+x+3/4,-y
-112 -x+1/2,+y+3/4,+z+1/4
-113 -y,-x+1/2,-z+1/2
-114 -z,-y+1/2,-x+1/2
-115 -x,-z+1/2,-y+1/2
-116 -y+3/4,-x+1/4,+z+1/2
-117 +z,-y+1/4,-x+1/4
-118 -x+3/4,+z+1/2,-y+1/4
-119 +z+3/4,-y,+x+3/4
-120 +x+1/4,+z+1/4,-y
-121 -x+1/2,+z+1/4,+y+3/4
-122 +y+1/4,-x,+z+1/4
-123 +z+3/4,+y+3/4,-x
-124 -y+1/2,+x+3/4,+z+1/4
201 +x+1/2,+y,+z+1/2
202 +z+1/2,+x,+y+1/2
203 +y+1/2,+z,+x+1/2
204 +x+3/4,+y+1/4,-z+1/2
205 -z+1/2,+x+1/4,+y+3/4
206 +y+3/4,-z,+x+3/4
207 -z+3/4,+x+1/2,-y+1/4
208 -y+1/4,-z+1/4,+x
209 +y,-z+1/4,-x+1/4
210 -x+1/4,+y+1/2,-z+3/4
211 -z+3/4,-x+3/4,+y
212 +x,-y+3/4,-z+3/4
213 +y+1/2,+x,+z+1/2
214 +z+1/2,+y,+x+1/2
215 +x+1/2,+z,+y+1/2
216 +y+3/4,+x+1/4,-z+1/2
217 -z+1/2,+y+1/4,+x+3/4
218 +x+3/4,-z,+y+3/4
219 -z+3/4,+y+1/2,-x+1/4
220 -x+1/4,-z+1/4,+y
221 +x,-z+1/4,-y+1/4
222 -y+1/4,+x+1/2,-z+3/4
223 -z+3/4,-y+3/4,+x
224 +y,-x+3/4,-z+3/4
-201 -x+1/2,-y,-z+1/2
-202 -z+1/2,-x,-y+1/2
-203 -y+1/2,-z,-x+1/2
-204 -x+1/4,-y+3/4,+z+1/2
-205 +z+1/2,-x+3/4,-y+1/4
-206 -y+1/4,+z,-x+1/4
-207 +z+1/4,-x+1/2,+y+3/4
-208 +y+3/4,+z+3/4,-x
-209 -y,+z+3/4,+x+3/4
-210 +x+3/4,-y+1/2,+z+1/4
-211 +z+1/4,+x+1/4,-y
-212 -x,+y+1/4,+z+1/4
-213 -y+1/2,-x,-z+1/2
-214 -z+1/2,-y,-x+1/2
-215 -x+1/2,-z,-y+1/2
-216 -y+1/4,-x+3/4,+z+1/2
-217 +z+1/2,-y+3/4,-x+1/4
-218 -x+1/4,+z,-y+1/4
-219 +z+1/4,-y+1/2,+x+3/4
-220 +x+3/4,+z+3/4,-y
-221 -x,+z+3/4,+y+3/4
-222 +y+3/4,-x+1/2,+z+1/4
-223 +z+1/4,+y+1/4,-x
-224 -y,+x+1/4,+z+1/4
301 +x+1/2,+y+1/2,+z
302 +z+1/2,+x+1/2,+y
303 +y+1/2,+z+1/2,+x
304 +x+3/4,+y+3/4,-z
305 -z+1/2,+x+3/4,+y+1/4
306 +y+3/4,-z+1/2,+x+1/4
307 -z+3/4,+x,-y+3/4
308 -y+1/4,-z+3/4,+x+1/2
309 +y,-z+3/4,-x+3/4
310 -x+1/4,+y,-z+1/4
311 -z+3/4,-x+1/4,+y+1/2
312 +x,-y+1/4,-z+1/4
313 +y+1/2,+x+1/2,+z
314 +z+1/2,+y+1/2,+x
315 +x+1/2,+z+1/2,+y
316 +y+3/4,+x+3/4,-z
317 -z+1/2,+y+3/4,+x+1/4
318 +x+3/4,-z+1/2,+y+1/4
319 -z+3/4,+y,-x+3/4
320 -x+1/4,-z+3/4,+y+1/2
321 +x,-z+3/4,-y+3/4
322 -y+1/4,+x,-z+1/4
323 -z+3/4,-y+1/4,+x+1/2
324 +y,-x+1/4,-z+1/4
-301 -x+1/2,-y+1/2,-z
-302 -z+1/2,-x+1/2,-y
-303 -y+1/2,-z+1/2,-x
-304 -x+1/4,-y+1/4,+z
-305 +z+1/2,-x+1/4,-y+3/4
-306 -y+1/4,+z+1/2,-x+3/4
-307 +z+1/4,-x,+y+1/4
-308 +y+3/4,+z+1/4,-x+1/2
-309 -y,+z+1/4,+x+1/4
-310 +x+3/4,-y,+z+3/4
-311 +z+1/4,+x+3/4,-y+1/2
-312 -x,+y+3/4,+z+3/4
-313 -y+1/2,-x+1/2,-z
-314 -z+1/2,-y+1/2,-x
-315 -x+1/2,-z+1/2,-y
-316 -y+1/4,-x+1/4,+z
-317 +z+1/2,-y+1/4,-x+3/4
-318 -x+1/4,+z+1/2,-y+3/4
-319 +z+1/4,-y,+x+1/4
-320 +x+3/4,+z+1/4,-y+1/2
-321 -x,+z+1/4,+y+1/4
-322 +y+3/4,-x,+z+3/4
-323 +z+1/4,+y+3/4,-x+1/2
-324 -y,+x+3/4,+z+3/4
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Os OS1 0.0 0.0 0.0 1.0 Uani 0.00247 16
Rb RB2 0.375 0.375 0.375 1.0 Uani 0.03413 8
O O3 0.3168(2) 0.125 0.125 1.0 Uani 0.00902 48
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 OS1 O3 180.0 105_544 . 111_443 n
O3 OS1 O3 91.74(7) 105_544 . 117_544 n
O3 OS1 O3 88.26(7) 105_544 . 119_443 n
O3 OS1 O3 91.74(7) 105_544 . 218_454 n
O3 OS1 O3 88.26(7) 105_544 . 220_353 n
O3 OS1 O3 88.26(7) 111_443 . 117_544 n
O3 OS1 O3 91.74(7) 111_443 . 119_443 n
O3 OS1 O3 88.26(7) 111_443 . 218_454 n
O3 OS1 O3 91.74(7) 111_443 . 220_353 n
O3 OS1 O3 180.0 117_544 . 119_443 n
O3 OS1 O3 91.74(7) 117_544 . 218_454 n
O3 OS1 O3 88.26(7) 117_544 . 220_353 n
O3 OS1 O3 88.26(7) 119_443 . 218_454 n
O3 OS1 O3 91.74(7) 119_443 . 220_353 n
O3 OS1 O3 180.0 218_454 . 220_353 n
RB2 RB2 RB2 109.4712(4) 4_556 . -7_555 n
RB2 RB2 RB2 109.47120(20) 4_556 . -8_645 n
RB2 RB2 RB2 109.47120(20) 4_556 . -11_555 n
RB2 RB2 O3 125.26440(20) 4_556 . 106_554 n
RB2 RB2 O3 125.26440(10) 4_556 . 116_545 n
RB2 RB2 O3 54.73560(10) 4_556 . -101_554 n
RB2 RB2 O3 54.73560(20) 4_556 . -108_555 n
RB2 RB2 O3 54.73560(10) 4_556 . -122_564 n
RB2 RB2 O3 125.26440(10) 4_556 . 204_455 n
RB2 RB2 RB2 109.47120(20) -7_555 . -8_645 n
RB2 RB2 RB2 109.47120(20) -7_555 . -11_555 n
RB2 RB2 O3 125.26440(20) -7_465 . 106_554 n
RB2 RB2 O3 54.73560(10) -7_465 . 116_545 n
RB2 RB2 O3 125.26440(10) -7_465 . -101_554 n
RB2 RB2 O3 54.73560(20) -7_465 . -108_555 n
RB2 RB2 O3 125.26440(10) -7_465 . -122_564 n
RB2 RB2 O3 54.73560(10) -7_465 . 204_455 n
RB2 RB2 RB2 109.4712(4) -8_645 . -11_555 n
RB2 RB2 O3 54.73560(20) -8_555 . 106_554 n
RB2 RB2 O3 54.73560(10) -8_555 . 116_545 n
RB2 RB2 O3 54.73560(10) -8_555 . -101_554 n
RB2 RB2 O3 125.26440(20) -8_555 . -108_555 n
RB2 RB2 O3 125.26440(10) -8_555 . -122_564 n
RB2 RB2 O3 125.26440(10) -8_555 . 204_455 n
RB2 RB2 O3 54.73560(20) -11_465 . 106_554 n
RB2 RB2 O3 125.26440(10) -11_465 . 116_545 n
RB2 RB2 O3 125.26440(10) -11_465 . -101_554 n
RB2 RB2 O3 125.26440(20) -11_465 . -108_555 n
RB2 RB2 O3 54.73560(10) -11_465 . -122_564 n
RB2 RB2 O3 54.73560(10) -11_465 . 204_455 n
O3 RB2 O3 90.0 106_554 . 116_545 n
O3 RB2 O3 90.0 106_554 . -101_554 n
O3 RB2 O3 180.0 106_554 . -108_555 n
O3 RB2 O3 90.0 106_554 . -122_564 n
O3 RB2 O3 90.0 106_554 . 204_455 n
O3 RB2 O3 90.0 116_545 . -101_554 n
O3 RB2 O3 90.0 116_545 . -108_555 n
O3 RB2 O3 180.0 116_545 . -122_564 n
O3 RB2 O3 90.0 116_545 . 204_455 n
O3 RB2 O3 90.0 -101_554 . -108_555 n
O3 RB2 O3 90.0 -101_554 . -122_564 n
O3 RB2 O3 180.0 -101_554 . 204_455 n
O3 RB2 O3 90.0 -108_555 . -122_564 n
O3 RB2 O3 90.0 -108_555 . 204_455 n
O3 RB2 O3 90.0 -122_564 . 204_455 n
OS1 O3 OS1 138.58(10) 4_555 . 6_555 n
OS1 O3 RB2 110.71(5) 4_555 . -8_645 n
OS1 O3 RB2 110.71(5) 6_555 . -8_645 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
OS1 RB2 4.193010(20) . 7_545 n
OS1 RB2 4.193010(20) . 8_554 n
OS1 RB2 4.193010(20) . 11_554 n
OS1 RB2 4.193010(20) . -7_454 n
OS1 RB2 4.193010(20) . -8_445 n
OS1 RB2 4.193010(20) . -11_445 n
OS1 O3 1.9114(6) . 105_544 n
OS1 O3 1.9114(6) . 111_555 n
OS1 O3 1.9114(6) . 117_544 n
OS1 O3 1.9114(6) . 119_555 n
OS1 O3 1.9114(6) . 218_454 n
OS1 O3 1.9114(6) . 220_555 n
RB2 OS1 4.193010(20) . 4_555 n
RB2 OS1 4.193010(20) . 5_555 n
RB2 OS1 4.193010(20) . 6_555 n
RB2 OS1 4.193010(20) . 7_555 n
RB2 OS1 4.193010(20) . 8_555 n
RB2 OS1 4.193010(20) . 9_555 n
RB2 OS1 4.193010(20) . 10_555 n
RB2 OS1 4.193010(20) . 11_555 n
RB2 OS1 4.193010(20) . 12_555 n
RB2 OS1 4.193010(20) . 101_555 n
RB2 OS1 4.193010(20) . 201_555 n
RB2 OS1 4.193010(20) . 301_555 n
RB2 RB2 4.379460(20) . 4_556 n
RB2 RB2 4.379460(20) . -7_455 n
RB2 RB2 4.379460(20) . -8_545 n
RB2 RB2 4.379460(20) . -11_455 n
RB2 O3 3.62388(28) . 1_555 n
RB2 O3 3.62388(28) . 2_555 n
RB2 O3 3.62388(28) . 3_555 n
RB2 O3 3.62388(28) . 9_555 n
RB2 O3 3.62388(28) . 10_555 n
RB2 O3 3.62388(28) . 11_555 n
RB2 O3 3.62388(28) . 19_555 n
RB2 O3 3.62388(28) . 20_555 n
RB2 O3 3.62388(28) . 24_555 n
RB2 O3 3.62388(28) . 101_555 n
RB2 O3 3.1167(17) . 106_554 n
RB2 O3 3.62388(28) . 108_555 n
RB2 O3 3.1167(17) . 116_545 n
RB2 O3 3.62388(28) . 122_555 n
RB2 O3 3.1167(17) . -101_644 n
RB2 O3 3.1167(17) . -108_545 n
RB2 O3 3.1167(17) . -122_554 n
RB2 O3 3.1167(17) . 204_455 n
O3 OS1 1.9114(6) . 4_555 n
O3 OS1 1.9114(6) . 6_555 n
O3 RB2 3.62388(28) . 1_555 n
O3 RB2 3.62388(28) . 8_554 n
O3 RB2 3.1167(17) . -8_545 n
